TOPIC PHASE DIAGRAMS

Document Sample

```					             PHASE DIAGRAMS
Phase A                                                   Phase B

Silver atom
Copper         atom

• When we combine two elements...
what equilibrium state do we get?
• In particular, if we specify...
--a composition (e.g., wt%Cu - wt%Ag), and
--a temperature (T)
THE SOLUBILITY LIMIT
• Solubility Limit:
Max concentration for which only a solution occurs.
(No precipitate)

• Ex: Phase Diagram: Water-Sugar System

Question: What is the solubility limit at 20C?

If Comp < 65wt% sugar: syrup
If Comp > 65wt% sugar: syrup + sugar coexist

• Solubility limit increases with T:
e.g., if T = 100C, solubility limit = 80wt% sugar.
Solubility Limit

3
EFFECT OF T & COMPOSITION (Co)
• Each point on this phase diagram represents equilibrium
• Changing T can change # of phases: path A to B
• Changing Co can change # of phases: path B to C

B
C

A
WATER-SALT PHASE DIAGRAM
Solubility limit

Reduction in
freezing point
COMPONENTS AND PHASES
• Components:
The elements or compounds which are mixed initially
(e.g., Al and Cu, or water and sugar)
• Phases:
The physically and chemically distinct material regions
that result (e.g.,  and , or syrup and sugar)

Aluminum-
Copper
Alloy

Fig. 9.0,
Callister 3e.
PHASE DIAGRAMS
• Tell us about phases as function of T, Co, P
• For this course:
--binary systems: just 2 components.
--independent variables: T and Co (P = 1 atm is always used)

• Phase
Diagram for Cu-
Ni system

• Isomorphous
system: i.e.,
complete solubility
of one                                        Adapted from Fig. 9.2(a), Callister 6e.
component in                                  (Fig. 9.2(a) is adapted from Phase
another                                       Diagrams of Binary Nickel Alloys, P.
Nash (Ed.), ASM International, Materials
Park, OH (1991).
Note change in
melting point
PHASE DIAGRAMS: # and types of phases
• Rule 1: If we know T and Co, then we know:
--the # and types of phases present.

• Examples:
A:
1 phase ()

B:
2 phases (L + )

Cu-Ni
phase
diagram
PHASE DIAGRAMS: composition of phases
• Rule 2: If we know T and Co, then we know:
--the composition of each phase.             Cu-Ni
system
Examples:
• C0 = 35 wt% Ni
• At 1300 C:
– Only liquid (L)
– CL = C0 (= 35 wt% Ni)
• At 1150 C:
– Only solid ()
– C = C0 (= 35 wt% Ni)
• At TB:
– Both  and L
– CL = Cliquidus (= 32 wt% Ni)
– C = Csolidus (=43 wt% Ni)
PHASE DIAGRAMS: weight fractions of phases
• Rule 3: If we know T and Co, then we know:
--the amount of each phase (given in wt%).               Cu-Ni
• C0 = 35 wt% Ni                                           system
• At 1300 C:
– Only liquid (L)
– WL = 100 wt%, W = 0 wt%
• At 1150 C:
– Only solid ()
– WL = 0 wt%, W = 100 wt%
• At TB:
– Both  and L
– WL = S/(R+S) =
(43-35)/(43-32) = 73 wt%
– W = R/(R+S) =
(35-32)/(43-32) = 27 wt%
The lever rule    10
THE LEVER RULE: A PROOF
• Sum of weight fractions:
• Conservation of mass (Ni):
• Combine above equations:

• A geometric interpretation:
COOLING A Cu-Ni BINARY
• System is:
--binary
i.e., 2 components:
Cu and Ni.
--isomorphous
i.e., complete
solubility of one
component in
another;  phase
field extends from
0 to 100wt% Ni.
• Consider
Co = 35wt%Ni.
• Equilibrium cooling
12
NON-EQUILIBRIUM PHASES
• C changes as we solidify.
• Cu-Ni case: First  to solidify has C = 46wt%Ni.
Last  to solidify has C = 35wt%Ni.
• Fast rate of cooling:             • Slow rate of cooling:
Cored structure                      Equilibrium structure
MECHANICAL PROPERTIES: Cu-Ni System
• Effect of solid solution strengthening on:
--Tensile strength (TS)                    --Ductility (%EL,%AR)

Adapted from Fig. 9.5(a), Callister 6e.   Adapted from Fig. 9.5(b), Callister 6e.
BINARY-EUTECTIC SYSTEMS
has a special composition
2 components                   with a min. melting T.
Cu-Ag
Ex.: Cu-Ag system                                         system
• 3 single phase regions
(L,  )
• Limited solubility:
 : FCC, mostly Cu
 FCC, mostly Ag
:
• T E: No liquid below TE
• CE: Min. melting T
composition
• 3 two phase regions
• Cooling along dotted
line:                            Callister 6e. (Fig. 9.6 adapted
from Binary Phase Diagrams, 2nd ed., Vol. 1, T.B.
L (71.9%)   (8%) +  (91.2%)   Massalski (Editor-in-Chief), ASM International, Materials
Park, OH, 1990.)
EX: Pb-Sn EUTECTIC SYSTEM (1)
• For a 40wt%Sn-60wt%Pb alloy at 150C, find...
Pb-Sn
--the phases present                                                system

--the compositions of
the phases

--the relative amounts
of each phase

from Binary Phase Diagrams, 2nd ed., Vol. 3, T.B.
Massalski (Editor-in-Chief), ASM International, Materials
Park, OH, 1990.)
EX: Pb-Sn EUTECTIC SYSTEM (2)
• For a 40wt%Sn-60wt%Pb alloy at 150C, find...
--the phases present:                                               Pb-Sn
+                                                           system
--the compositions of
the phases:
C = 11wt%Sn
C = 99wt%Sn
--the relative amounts
of each phase:
(lever rule)

from Binary Phase Diagrams, 2nd ed., Vol. 3, T.B.
Massalski (Editor-in-Chief), ASM International, Materials
Park, OH, 1990.)
MICROSTRUCTURES
IN EUTECTIC SYSTEMS-I
• Co < 2wt%Sn

• Result:
--polycrystal of  grains.

Callister 6e.
MICROSTRUCTURES
IN EUTECTIC SYSTEMS-II
• 2wt%Sn < Co < 18.3wt%Sn

• Result:
-- polycrystal with fine
 crystals.

Pb-Sn
system

Callister 6e.
MICROSTRUCTURES
IN EUTECTIC SYSTEMS-III
• Co = CE (Eutectic composition)
• Result: Eutectic microstructure
--alternating layers of  and  crystals.

Pb-Sn
system

Adapted from Fig. 9.12, Callister 6e.
(Fig. 9.12 from Metals Handbook, Vol.
9, 9th ed., Metallography and
Microstructures, American Society for
Metals, Materials Park, OH, 1985.)
Callister 6e.
MICROSTRUCTURES
IN EUTECTIC SYSTEMS-IV
• 18.3wt%Sn < Co < 61.9wt%Sn
• Result:  crystals and a eutectic microstructure

Pb-Sn
system

Callister 6e.
HYPOEUTECTIC & HYPEREUTECTIC

Callister 6e. (Fig. 9.7
Phase Diagrams, 2nd ed.,
Vol. 3, T.B. Massalski
(Editor-in-Chief), ASM
International, Materials
Park, OH, 1990.)

(Figs. 9.12 and 9.15
from Metals
Handbook, 9th ed.,
Vol. 9,
Metallography and
Microstructures,
American Society
for Metals, Materials
Park, OH, 1985.)

Fig. 9.15, Callister 6e.   Adapted from Fig. 9.12,   Callister 6e. (Illustration
Callister 6e.             only)
COMPLEX PHASE DIAGRAMS: Cu-Zn
IRON-CARBON (Fe-C) PHASE DIAGRAM

• Pure iron: 3 solid
phases
– BCC ferrite ()
– FCC Austenite ()
– BCC 
• Beyond 6.7% C
cementite (Fe3C)
• Eutectic: 4.3% C
– L   + Fe3C
– (L  solid + solid)
• Eutectoid: 0.76% C
–    + Fe3C
– (solid  solid +
solid)
Fe-C PHASE DIAGRAM: EUTECTOID
POINT

Pearlite microstructure:
Just below the eutectoid
point
EUTECTOID POINT: LEVER RULE

• Just below the
eutectoid point:

• W = (6.7-0.76)/(6.7-
0.022) = 89%

• WFe3C = (0.76-
0.022)/(6.7-0.022) =
11%
HYPOEUTECTOID STEEL

Proeutectoid :
 phase formed at T > Teutectoid
HYPEREUTECTOID STEEL
ALLOYING STEEL WITH MORE ELEMENTS

• Teutectoid changes:                               • Ceutectoid changes:

Adapted from Fig. 9.31,Callister 6e. (Fig. 9.31     Adapted from Fig. 9.32,Callister 6e. (Fig. 9.32
from Edgar C. Bain, Functions of the Alloying       from Edgar C. Bain, Functions of the Alloying
Elements in Steel, American Society for Metals,     Elements in Steel, American Society for Metals,
1939, p. 127.)                                      1939, p. 127.)
SUMMARY
• Phase diagrams are useful tools to determine:
--the number and types of phases,
--the wt% of each phase,
--and the composition of each phase
for a given T and composition of the system.
• Alloying to produce a solid solution usually
--increases the tensile strength (TS)
--decreases the ductility.
• Binary eutectics and binary eutectoids allow for
a range of microstructures.

```
DOCUMENT INFO
Shared By:
Categories:
Stats:
 views: 9 posted: 5/1/2011 language: English pages: 30